Mechanically robust electrospun hydrogel scaffolds crosslinked … · Mechanically robust...
Embed Size (px)
Transcript of Mechanically robust electrospun hydrogel scaffolds crosslinked … · Mechanically robust...
Mechanically robust electrospun hydrogel scaffoldscrosslinked via supramolecular interactionsCitation for published version (APA):Mollet, B. B., Spaans, S., Goodarzy Fard, P., Bax, N. A. M., Bouten, C. V. C., & Dankers, P. Y. W. (2017).Mechanically robust electrospun hydrogel scaffolds crosslinked via supramolecular interactions. MacromolecularBioscience, 17(9), . https://doi.org/10.1002/mabi.201700053
Document status and date:Published: 01/09/2017
Document Version:Accepted manuscript including changes made at the peer-review stage
Please check the document version of this publication:
• A submitted manuscript is the version of the article upon submission and before peer-review. There can beimportant differences between the submitted version and the official published version of record. Peopleinterested in the research are advised to contact the author for the final version of the publication, or visit theDOI to the publisher's website.• The final author version and the galley proof are versions of the publication after peer review.• The final published version features the final layout of the paper including the volume, issue and pagenumbers.Link to publication
General rightsCopyright and moral rights for the publications made accessible in the public portal are retained by the authors and/or other copyright ownersand it is a condition of accessing publications that users recognise and abide by the legal requirements associated with these rights.
• Users may download and print one copy of any publication from the public portal for the purpose of private study or research. • You may not further distribute the material or use it for any profit-making activity or commercial gain • You may freely distribute the URL identifying the publication in the public portal.
If the publication is distributed under the terms of Article 25fa of the Dutch Copyright Act, indicated by the “Taverne” license above, pleasefollow below link for the End User Agreement:www.tue.nl/taverne
Take down policyIf you believe that this document breaches copyright please contact us at:[email protected] details and we will investigate your claim.
Download date: 08. Feb. 2021
- 1 -
DOI: 10.1002/marc.((insert number)) ((or ppap., mabi., macp., mame., mren., mats.)) Full Paper Mechanically robust electrospun hydrogel scaffolds crosslinked via supramolecular interactions Björne B. Mollet, Sergio Spaans, Parinaz Goodarzy Fard, Noortje A.M. Bax, Carlijn V.C. Bouten, Patricia Y.W. Dankers* ––––––––– Dr. B.B. Mollet Institute for Complex Molecular Systems and Laboratory of Chemical Biology Department of Biomedical Engineering Eindhoven University of Technology, P.O. Box 513, 5600 MB Eindhoven, Netherlands E-mail: [email protected] MSc S. Spaans Institute for Complex Molecular Systems and Laboratory for Cell and Tissue Engineering, Department of Biomedical Engineering Eindhoven University of Technology, P.O. Box 513, 5600 MB Eindhoven, Netherlands E-mail: [email protected] BSc P. Goodarzy Fard Institute for Complex Molecular Systems and Laboratory of Chemical Biology Department of Biomedical Engineering Eindhoven University of Technology, P.O. Box 513, 5600 MB Eindhoven, Netherlands E-mail: [email protected] Dr. N.A.M. Bax Institute for Complex Molecular Systems and Laboratory for Cell and Tissue Engineering, Department of Biomedical Engineering Eindhoven University of Technology, P.O. Box 513, 5600 MB Eindhoven, Netherlands E-mail: [email protected] Prof. Dr. C.V.C. Bouten Institute for Complex Molecular Systems and Laboratory for Cell and Tissue Engineering, Department of Biomedical Engineering Eindhoven University of Technology, P.O. Box 513, 5600 MB Eindhoven, Netherlands E-mail: [email protected] Dr. Dr. P.Y.W. Dankers Institute for Complex Molecular Systems, Laboratory of Chemical Biology and Laboratory for Cell and Tissue Engineering Department of Biomedical Engineering Eindhoven University of Technology, P.O. Box 513, 5600 MB Eindhoven, Netherlands E-mail: [email protected] –––––––––
- 2 -
One of the major challenges in the processing of hydrogels based on poly(ethylene glycol)
(PEG) is to create mechanically robust electrospun hydrogel scaffolds without chemical cross-
linking post-processing. In this study, this was achieved by the introduction of physical
crosslinks in the form of supramolecular hydrogen bonding ureido-pyrimidinone (UPy)
moieties, resulting in chain-extended UPy-PEG polymers (CE-UPy-PEG) that could be
electrospun from organic solvent. The resultant fibrous meshes were swollen in contact with
water and formed mechanically stable, elastic hydrogels, while the fibrous morphology
remained intact. Mixing up to 30 wt% gelatin with these CE-UPy-PEG polymers introduced
bioactivity into these scaffolds, without affecting the mechanical properties. Manipulating the
electrospinning parameters resulted in meshes with either small or large fiber diameters, i.e.
0.63±0.36 µm and 2.14±0.63 µm, respectively. In that order, these meshes provided support
for renal epithelial monolayer formation or a niche for the culture of cardiac progenitor cells.
For regenerative medicine and tissue engineering purposes a diversity of biomaterial
hydrogels, ranging from natural to synthetic, have been described and studied,1–6 each with
their specific advantages and limitations. Hydrogels of natural origin, such as collagen or its
denatured form gelatin, hyaluronic acid, and matrigel, a widely applied commercial
extracellular matrix (ECM) mimic, all provide biological environments that promote cellular
survival and interaction with cells.7 However, the variable composition of these materials, and
their complex and not-well understood interactions with cells, challenge controlled
application. In addition, origin-related safety concerns put constraints on their use in the
medical field.8 On top of that, the possibility to tune the mechanical or topological properties
of these molecularly pre-defined hydrogels is limited. Inert synthetic hydrogels, on the other
- 3 -
hand, allow adjustable composition and hence predictable and tunable properties. However,
synthetic materials lack bioactive cues for engagement of specific interaction with cells. To
bridge the gap between natural and synthetic hydrogels, researchers have simply mixed
hydrogel components of natural and synthetic origin to achieve hybrid hydrogels with
To enable the formation of structurally defined, freestanding meshes, the hydrogel system
must allow processing and acquire mechanically robust properties. Electrospinning is an
attractive processing technique for the formation of fibrous meshes. By controlling fiber
diameter, the pore size can be tuned. This allows the formation of scaffolds either distinctly
suitable to function as 2D support, or 3D scaffolds that allow cell infiltration. Electrospinning
of natural,12,13 synthetic14–17 and hybrid18 hydrogelators has been performed extensively.
However, all these biomaterials require chemical cross-linking post-electrospinning to prevent
complete dissolution or fast degradation of the nano-to-micro fibrous structures in aqueous
environments and/or to improve poor mechanical properties. A hydrogel material that forms
strong physical cross-links could circumvent the need of chemical cross-linking, while
retaining the opportunity for processing.
Here we demonstrate the use of a supramolecular hydrogelator based on poly(ethylene glycol)
(PEG) with multiple ureido-pyrimidinone (UPy)-moieties in the backbone,19 electrospun into
mechanically strong, microfibrous meshes (Figure 1A). While this chain-extended UPy-PEG
(CE-UPy-PEG) has a nearly identical chemical composition compared to its telechelic
analogues, it exhibits completely different, exceptional mechanical properties.20–23 In the dry
state, this supramolecular polymer forms a tough material with shape memory properties,
whereas in the hydrated state a strong and highly elastic hydrogel is formed.19 In the
equilibrium hydrated state, the bulk hydrogel (with 10 kg · mol-1 PEG-block) contains ~85
wt% water. This hydrogel material showed nearly perfect strength recovery even at large
deformation (> 300%).19 Hence, the increased chain length, realized through chain-extension,
- 4 -
and the ability to form physical cross-links substantially enhanced the strength, ductility, and
stability of this material in water. Importantly, no chemical cross-linking is needed to achieve
these remarkable material properties while at the same time the physical cross-links, formed
by hydrogen-bonding between UPy-dimers, are reversible by nature. As such, these links can
be dissociated and reformed as desired in a controlled fashion, offering attractive processing
Based on these properties, CE-UPy-PEG was hypothesized to be well-suited as hydrogel
scaffold material for tissue engineering applications. To induce a cell adhesive character to
the bio-inert CE-UPy-PEG, mixing with a bioactive natural hydrogel component was
performed. For this purpose gelatin was chosen, due to its compatibility with electrospinning
processes.24–26 By incorporation of gelatin in the electrospinning process, we demonstrate the
use of this hydrogel scaffold to support the formation of renal monolayers and as a cardiac
progenitor cell niche.
2. Experimental Section
Chain-extended ureido-pyrimidinone functionalized poly(ethylene glycol) (CE-UPy-PEG)
with Mn,PEG = 10 kg mol-1 was synthesized as previously described.19 As a consequence of the
high polydispersity index (PDI >3) the number of repeats, or UPy-functionalities, per
macromolecular monomer was estimated to be around 50 repeats on average based on average
molecular weight determined by GPC. Gelatin type A, derived from porcine skin with ~300 g
Bloom gel strength, and 1,1,1,3,3,3-hexafluoro-2-propanol (HFIP) were purchased from
- 5 -
2.2. Electrospun meshes
2.2.1 Small fiber diameters
Viscous solutions (5 wt/v%) of different weight ratios of CE-UPy-PEG/gelatin, i.e. 100/0,
90/10, 80/20, 70/30, were prepared by dissolving 200 mg solid material in 4 mL HFIP. First
the CE-UPy-PEG fraction was dissolved in HFIP, after which gelatin was added and the
solutions were stirred at room temperature overnight. The clear viscous solution was
transferred to a 2.5 mL glass syringes (Hamilton) and fed at 50 μL min-1 using a syringe pump
(KR analytical) at the outside of the electrospinning cabinet to the flat-tip stainless-steel 23G
needle (Intertronics) inside the cabinet, via a ~35 cm long 1 mm I.D. PTFE tube. Inside the
cabinet, each solution was spun with an in-house built electrospun setup by the application of
18.5 kV between a tip-to-target distance of 12 cm. To enable facile removal of the non-woven
electrospun mesh, the collector was covered with a thin sheet of polyethylene film. To
provide a flat surface and extra support to thin samples of the electrospun mesh, fibers were
collected on 12 mm round glass coverslips. The fiber deposition was interrupted several times
to move the static collector plate over a 3x3 grid to enlarge the area of fiber deposition and to
achieve a more homogeneous mesh thickness. The electrospun mesh was gently removed
from the collector plate together with the polyethylene film and placed in vacuo at 40 °C to
remove any residual solvent overnight.
2.2.2 Large fiber diameters
A more viscous solution (10 wt/v%) of 80/20 CE-UPy-PEG/gelatin in HFIP was prepared by
dissolving 400 mg CE-UPy-PEG and 100 mg gelatin in 5 mL HFIP and stirred at 40 °C
overnight. The clear viscous solution was transferred to a syringe and connected via a 1 mm
I.D. PTFE tube and a 19G needle to the climate controlled electrospinning apparatus (IME
Technologies) set at 22-23 °C and 25% humidity. The solution was fed at 75 µL min-1, spun
- 6 -
by 12 kV with a tip-to-target distance of 12 cm and collected during an hour at an aluminum
foil covered rotating drum with 28 mm diameter, rotating at 100 rpm. The electrospun mesh
was placed in vacuo at 40 °C to remove any residual solvent overnight. The thickness of the
collected CE-UPyPEG/gelatin mesh in dry state, measured with an automatic ruler, was 300
2.3. Environmental scanning electron microscopy (ESEM)
Environmental scanning electron microscopy (ESEM) imaging was performed by using FEI
Quanta 600F and Xt Microscope Control software. Samples were prepared by placing small
pieces of each mesh on double-sided sticky carbon tape on a metal stub. The uncoated
samples were visualized under low vacuum (~0.5 mbar) with an accelerating voltage of 15-20
kV and a working distance of 6.9-8.2 mm. Images were recorded up to 10,000 times
magnification. In low vacuum, both backscattering electrons and secondary electrons were
detected. Electrospun meshes with thick fibers were imaged using ESEM at high vacuum,
with a voltage of 1 kV, working distance of 10 mm and spot size of 3.0 mm. Fiber diameters
were determined from multiple high magnification images using ImageJ software and
expressed as average ± standard deviation.
2.4 Fluorescence microscopy visualisation of gelatin distribution
Prewet CE-UPy-PEG hydrogel samples on glass, both drop-cast films and electrospun meshes
with varying gelatin content, were incubated overnight at 37 °C with a solution of
CNA35mTurquoise2 in PBS at a concentration of 1 µM.27 Samples were washed once with
PBS before imaging with fluorescence microscopy (Zeiss Axio Observer D1) with λex = 426-
446 nm and λem = 460-500 nm.
- 7 -
2.4. Biaxial mechanical testing of electrospun meshes
The mechanical performances of CE-UPy-PEG electrospun meshes, both with and without
gelatin, were measured. Square samples of approximately 8 x 8 mm were cut from the
meshes. The samples were weighed before and after hydration to gain insight into the
swelling behavior and the thickness was determined using a digital microscope (Keyence,
VHX-500F). The hydrated sample was mounted in a biaxial tensile testing device equipped
with 1.5 N load cells (CellScale), as illustrated in Figure S1. Four rakes (BioRake Delicate,
0.7 mm, 30 mm, CellScale) each consisting of five metal hooks with a diameter of 250 µm,
were attached to the dry sample, leading to a 3500 x 3500 µm square testing area. The sample
was emerged in a water bath, which was maintained at 37 °C, during the straining protocol.
For determination of elastic moduli and confirmation of isotropic behavior of the meshes with
randomly oriented fibers, the meshes were cyclically loaded with three repeats of uniaxial
stretch in both x and y direction, and three repeats of equibiaxial stretch. Stretch was applied
at a rate of 2% s-1 and each final stretch was applied for 2 s. Between cycles, the sample was
not loaded for 5 s to allow the fibers to relax and return to their initial configuration. The
applied stretch was increased after each set of cycles starting at 10% up to 50% with
increments of 10%. During the whole protocol, images were taken with a camera at a
frequency of 1 Hz, while numerical data, i.e global stretch, or displacement in µm and force in
mN, was generated at a frequency of 30 Hz. The images were used as reference for visual
control of sample integrity. Data was converted with Matlab (Mathworks) to calculate stresses
and matched with the applied strains. In these calculations, the surface was determined by
multiplying the thickness of the hydrated sample with 3500 μm, thereby assuming a uniform
solid material. As the signal to noise ratio for the measured forces was low, the average stress
was determined per second from the redundant data acquisition frequency. In determining the
moduli via Hook’s law, linear-elastic behavior of the materials was assumed. Per sample the
- 8 -
elastic modulus was determined for both x- and y-direction via a linear fit through the
corresponding part of the uniaxial stress-strain curve derived from a 20 or 30% stretch cyclus,
upon which the average was used in determining the modulus per material.
2.5. Renal epithelial cell culture
Human Kidney-2 (HK-2) cells, an immortalized proximal tubule epithelial cell line,28 were
routinely cultured in polystyrene culture flaks (BD Falcon) in complete medium consisting of
Dulbecco’s Modified Eagle Medium (DMEM, Gibco) supplemented with 10% heat
inactivated fetal bovine serum (26140-079, Gibco, Invitrogen) and 1% penicillin-streptomycin
solution (Gibco, Invitrogen), at 37 °C and 5% CO2 in a humidified atmosphere. Cells were
passed when they were 80-90% confluent. Circular samples of 12 mm, supported by a glass
coverslip, were cut from the electrospun meshes (small fiber diameter). Samples were
sterilized via UV-irradiation (Osram, HNS 30W G13, 13.4 W radiated power UVC 200-280
nm, with 90% of relative spectral radial power at 254 nm) for 1 hour on each side at a
distance of 10-20 cm, inside a lamellar airflow cabinet and fixed in dry state in minusheet
tissue carriers with an outer diameter of 13 mm (Minucells and Minutissue vertriebs gmbh) or
adapted transwell culture systems (BD Biosciences). The carriers with samples were placed in
a 24-well tissue culture plate (BD Biosciences). Each mesh sample was submerged in an
ample volume of complete medium, which was removed right before cell seeding. For low
cell density, 55 x 103 HK-2 were seeded, and for high cell density, 100 x 103 HK-2 were
seeded and cultured at 37° C and 5 % CO2. The low density cell cultures were sacrificed after
1 day and actin, vincullin and cell nuclei were stained. High cell density cultures were
sacrificed after 3 days and zona occludens-1 (ZO-1) and cell nuclei were stained (See
- 9 -
2.6. Cardiomyocyte progenitor cell culture
Cardiomyocyte progenitor cells (CMPC), immortalized via a lentiviral transduction,29 were
routinely cultured in polystyrene culture flasks pre-coated with 0.1 wt/v% gelatin (Sigma) in
PBS. CMPC were cultured in SP++ growth medium (GM) consisting of M199
(Gibco)/EGM2 medium (3:1) supplemented with 10% fetal bovine serum (FBS), 1%
penicillin/streptomycin (Lonza DE17-602E) and 1% non-essential amino acids (Gibco).
CMPC were passaged when they were 80-90% confluent. Electrospun meshes with large fiber
diameter were cut in circular samples with a diameter of 12 mm and sterilized via UV-
irradiation (GE, NPP 130 LPF 30W G13) for 1 hour on each side at a distance of 10-20 cm,
inside a lamellar airflow cabinet. Meshes were then fixed in dry state in minusheet tissue
carriers with an outer diameter of 13 mm (Minucells and Minutissue vertriebs gmbh). CMPC
were seeded into the scaffold (250 x 103 or 1000 x 103 cells per mesh) by centrifugal force
according to a previously described method.30 Cultures were analyzed at day 1 and day 9 with
Live/Dead staining or sacrificed after 1 day for immunofluorescent staining of cardiac-
specific ECM components (See Supporting Information).
3. Results and Discussion
3.1. Electrospun CE-UPy-PEG meshes
Electrospinning of the CE-UPy-PEG polymer resulted in the formation of randomly oriented
fibers with diameters typically of 0.68±0.23 µm in the dry state (Figure 1B and C, state I).
Upon contact with water, the white, opaque meshes hydrated and formed semi-transparent
hydrogel scaffolds (Figure 1B, state II). The meshes could take up over 12 times their dry
weight in water (~93 wt%). This was much more compared to the bulk CE-UPy-PEG
material, which was determined to take up ~5.7 times its dry weight in water (~85 wt%) in
- 10 -
equilibrated hydrated state.19 This difference is attributed to the porous structure of the mesh.
Upon hydration, the fibers swell, but also the empty spaces between them become completely
filled with water as a result of capillary force. In contrast to bulk material, which swells
proportionally equal in all directions, the meshes appeared to swell primarily in the height and
less in the planar direction of the electrospun mesh (Figure 1B, state I and II). For individual
fibers collected on a glass substrate it could be clearly observed how contact with water
increased both fiber diameter and length upon hydration. Due to the high ratio between both
dimensions, the proportional swelling resulted in buckling of the fibers between contact points
(Figure 1B, state II and III). Hydrated samples of the mesh were dried and imaged by ESEM
to gain understanding of the effect of hydration on the mesh morphology at microscale
(Figure 1C, state III). Overall, the remaining fibrous structure was less well defined compared
to the original dry mesh as spun. Nevertheless, contours of individual fibers could still be
distinguished in the mesh. These results show that the CE-UPy-PEG polymer can be
electrospun into dry solid fibrous meshes that upon exposure to aqueous solution swell into
fibrous hydrogel structures. Subsequent drying of these hydrogel meshes resulted in a dry
electrospun mesh, showing that the process of mesh formation, swelling and hydrogel
formation, is reversible. Furthermore, degradability of CE-UPy-PEG should be addressed in
future research. Due to the ethylene glycol monomers, urethane and urea functionalities, it is
proposed that this mesh is prone to oxidative and enzymatic degradation in vivo.31
Introduction of bioactivity to the CE-UPy-PEG meshes was established by the addition of
gelatin in the electrospinning solution. Mixtures with different gelatin concentrations were
succesfully electrospun using the same electrospinning settings and resulted in meshes with
average fiber diameters of 0.68±0.23 µm (0 wt% gelatin), 0.63±0.36 µm (20 wt% gelatin),
and 0.65±0.39 µm (30 wt% gelatin) in the dry state. This indicated that the addition of gelatin
to CE-UPy-PEG did not induce significant changes to the electrospinning process. In
- 11 -
literature, increase in gelatin content has been described to reduce fiber diameters upon
electrospinning by the same conditions for mixtures with various synthetic polymers, e.g.
polycaprolactone (PCL),32,33 poly(L-lactide-co-ε-caprolactone) (PLCL),34 poly(lactic-co-
glycolic acid) (PLGA)35 and polyglycolic acid (PGA).36 However, up to 30 wt% gelatin could
be added to CE-UPy-PEG while maintaining similar mesh morphology and swelling
3.2. Mechanical testing
Elasticity and durability of a hydrogel scaffold is of high importance in for example
cardiovascular tissue engineering applications, which involve mechanical loading under
cyclic loading. The mechanical properties of electrospun scaffolds are highly dependent on
the processing parameters. Next to polymeric composition, also fiber diameter and orientation
are major factors that determine the elastic modulus of electrospun meshes.32 To gain
understanding of the mechanical properties of electrospun CE-UPy-PEG, hydrated meshes
were subjected to biaxial tensile tests (Figure S1). The effect of gelatin was determined by
comparison of meshes of CE-UPy-PEG with 0, 20 and 30 wt% gelatin (Figure 2A). As
expected, the random orientation of the fibers in these meshes, resulted in isotropic elastic
behavior in X and Y direction (Figure S2). Furthermore, stress-strain curves of meshes which
were stretched and relaxed in the x-direction showed overlap, which indicates minimal plastic
deformation within the applied range of strains (Figure 2B). Elastic moduli were determined
for pure CE-UPy-PEG meshes, and hybridized meshes with 20 and 30 % gelatin (Table 1).
Initial measurements did not reveal an influence of the addition of gelatin on the mechanical
properties of the meshes. All hydrogel meshes exhibited strain-to-failure of at least 40%. At
higher deformations, the material started to tear at the points where the mesh was punctured
with thin metal pins for attachment to the biaxial tensile testing device. When strains were
further increased, eventually total rupture always occurred along a row of these pins. At these
- 12 -
points in the material, locally higher stresses occur. Therefore, the currently derived elastic
moduli are probably underestimates as these were derived from global stress-strain curves.
However the strain-to-failure could be considered representative for applications that require
for example suturing of the hydrogel meshes. These results indicate that CE-UPy-PEG based
hydrogel meshes could potentially be applied in tissue engineering applications that involve
mechanical straining up to 30-40%.
3.3. Renal epithelial cell adhesion and monolayer formation
Renal epithelial cells did not adhere to drop-cast films solely consisting of CE-UPy-PEG
owing to the anti-fouling nature of PEG. The addition of gelatin to CE-UPy-PEG in the drop-
cast process only resulted in minor improvement of cell adhesion, which is proposed to occur
due to inhomogeneous mixing of gelatin into the CE-UPy-PEG (Figure S3-5). However,
when a mixed solution of CE-UPy-PEG and gelatin was processed by electrospinning, gelatin
was homogeneously distributed throughout each mesh (Figure 3A). Cells were first seeded in
sub-confluent densities on these meshes to enable focus on cell-biomaterial interactions rather
than cell-cell interactions. Cell adhesion was improved upon introduction of gelatin in the
electrospun mesh. Interestingly, formation of focal adhesions by attached renal epithelial cells
was identified via vinculin rich spots 1 day after cell seeding (Figure S6). The formation of
focal adhesions provides evidence for the interaction between cells and the hybrid mesh. This
thus confirmed the presence of the gelatin at the fibers surface and successful incorporation of
bioactivity through the use of gelatin in combination with electrospinning.
In order to create a tissue engineered renal cell monolayer, which can possibly be translated
towards an artificial kidney application,37 higher densities of renal epithelial cells were used.
The adhered cells were allowed to mature for 3 days prior to evaluation of their morphology
by fluorescence microscopy (Figure 3B). The presence of 10 wt% gelatin in the CE-UPy-PEG
mesh allowed some renal epithelial cells to adhere and grow in a patchy conformation. In
- 13 -
presence of 20 and 30 wt% gelatin the renal epithelial cells formed a near confluent layer
(Figure 3B). Staining of zona occludens-1 (ZO-1) protein and visualization by fluorescence
microscopy revealed the presence of tight junctions between the cells (Figure 3C). This points
towards the formation of a tight renal epithelial cell layer on this hybrid hydrogel mesh. These
results suggest suitability of the hybridized microfibrous hydrogels to function as scaffold to
support the formation of a confluent and functional renal cell monolayer.
3.4. CMPC viability and extracellular matrix production
Hybrid hydrogel meshes with a more open pore structure were hypothesized to provide a
suitable 3D environment for CMPC. The function of such a hydrogel is to maintain cell
viability and support growth and differentiation. It should hence act as a temporarily 3D
microenvironment which resembles the native niche until the cells have formed their own
ECM. Electrospinning a concentrated (10 wt/v%) solution of 80/20 wt/wt% CE-UPy-
PEG/gelatin resulted in a mesh with average fiber diameters of 2.14 ± 0.63 µm and apparent
pore sizes bigger than 10 µm (Figure 4A). Next, cardiomyocyte progenitor cells (CMPC)
were seeded inside the open porous structure of electrospun CE-UPy-PEG/gelatin meshes. To
actively aid cell infiltration, cells were forced into the mesh by centrifugation. Cell infiltration
depth in the hybrid CE-UPy-PEG/gelatin mesh increased after application of centrifugal force
compared to static seeding, with depths of 69 µm and 20 µm, respectively (Figure S7).
The viability of CMPC after 1 day of seeding was 97.5±0.5 % and after 9 days, cell viability
slightly decreased to 93.2±2.2 % (Figure S8). This is due to the thin electrospun meshes (300
µm in dry state), which allows for sufficient oxygen and nutrient to the cells. In addition, the
deposition of cardiac-specific ECM proteins by CMPC was determined by
immunofluorescent staining for collagen I, III, IV and fibronectin (Figure 4B). After 1 day of
culturing inside the hydrogel mesh, CMPC produced limited amounts of cytoplasmic collagen
I and IV. Co-staining of collagen III and membrane marker integrin β1 revealed the presence
- 14 -
of collagen III in the extracellular space. Furthermore, high amounts of fibronectin were
produced after 1 day. This fibronectin formed a fibrous structure at the attachment points with
the scaffold. One of the hurdles of hybrid hydrogels composed of a synthetic and natural
component is that the biological ECM component often degrades more rapid than its
replacement which is secreted by cells. Therefore, the deposition of ECM proteins by CMPC
shown here, is proposed to provide a promising start for successful long-term outcome.
These results show that hybrid hydrogel meshes based on CE-UPy-PEG can function as a
robust free-standing scaffold and support the formation of a renal cell monolayer and act as a
cardiac niche by simply tuning the fiber diameter. CE-UPy-PEG was successfully processed
by electrospinning into relevant fibrous morphologies, which are stable under physiological
conditions without the need of chemical cross-linking. The combination with gelatin
demonstrates the possibility to make hybrid scaffolds with natural bioactive proteins, while
synthetic UPy-peptide based approaches towards more specific and controlled bioactivation
might be explored in the future.38,39 The elastic behaviour of the hydrogel scaffolds and
durability under cyclic loading widens the scope of possible tissue engineering applications.
Anthal Smits is acknowledged for his support and guidance in the mechanical analysis of the
hybrid hydrogel meshes. Louis Pitet is thanked for the synthesis of the CE-UPy-PEG
polymer. Marie-José Goumans is gratefully acknowledged for the L9TB CMPC. The research
leading to these results has received funding from the ministry of Education, Culture and
Science (Gravity program 024.001.035), The Netherlands Organisation for Scientific
Research (NWO), the European Research Council (FP7/2007-2013), ERC Grant Agreement
- 15 -
308045. This research forms part of the Project P3.01 BioKid of the research program of the
Biomedical Materials institute, cofounded by the Dutch Ministry of Economic Affairs. The
financial contribution of the Dutch Kidney Foundation is gratefully acknowledged. Also, this
research forms part of the Cardiovasculair Onderzoek Nederland (CVON). The financial
contribution of the Nederlandse Hartstichting is gratefully acknowledged.
Received: Month XX, XXXX; Revised: Month XX, XXXX; Published online:
((For PPP, use “Accepted: Month XX, XXXX” instead of “Published online”)); DOI:
10.1002/marc.((insert number)) ((or ppap., mabi., macp., mame., mren., mats.))
Keywords: Supramolecular biomaterials, hybrid hydrogels, electrospun meshes, mechanical
properties, tissue engineering.
 Wang, R. M.; Christman, K. L. Adv. Drug Deliv. Rev. 2016, 96.
 van Marion, M.; Bax, N.; van Spreeuwel, A.; van der Schaft, D.; Bouten, C. Curr.
Pharm. Des. 2014, 20, 12.
 Bouten, C. V. C.; Dankers, P. Y. W.; Driessen-Mol, A.; Pedron, S.; Brizard, A. M. A.;
Baaijens, F. P. T. Adv. Drug Deliv. Rev. 2011, 63, 4–5.
 Drury, J. L.; Mooney, D. J. Biomaterials 2003, 24.
 Slaughter, B. V.; Khurshid, S. S.; Fisher, O. Z.; Khademhosseini, A.; A.Peppas, N.
Princ. Regen. Med. 2011.
 Radhakrishnan, J.; Krishnan, U. M.; Sethuraman, S. Biotechnol. Adv. 2014, 32, 2.
 Hughes, C. S.; Postovit, L. M.; Lajoie, G. a. Proteomics 2010, 10.
 Kleinman, H. K.; Martin, G. R. Semin. Cancer Biol. 2005, 15.
 Jia, X.; Kiick, K. L. Macromol. Biosci. 2009, 9, 2.
 Zhu, J.; Marchant, R. E. Expert Rev. Med. Devices 2011, 8, 5.
- 16 -
 Anjum, F.; Carroll, A.; Young, S. A.; Flynn, L. E.; Amsden, B. G. Macromol. Biosci.
2017, 201600373, 1600373.
 Matthews, J. A.; Wnek, G. E.; Simpson, D. G.; Bowlin, G. L. Biomacromolecules
2002, 3, 2.
 Liu, L.; Yoshioka, M.; Nakajima, M.; Ogasawara, A.; Liu, J.; Hasegawa, K.; Li, S.;
Zou, J.; Nakatsuji, N.; Kamei, K. ichiro; Chen, Y. Biomaterials 2014, 35, 24.
 Im, J. S.; Yun, J.; Lim, Y. M.; Kim, H. Il; Lee, Y. S. Acta Biomater. 2010, 6, 1.
 Stephens-Altus, J. S.; Sundelacruz, P.; Rowland, M. L.; West, J. L. J. Biomed. Mater.
Res. - Part A 2011, 98 A, 2.
 Gestos, A.; Whitten, P. G.; Wallace, G. G.; Spinks, G. M. Soft Matter 2012, 8, 31.
 Cay, A.; Mohsen Miraftab. J. Appl. Polym. Sci. 2013, 129, 6.
 Kim, K.-O.; Akada, Y.; Kai, W.; Kim, B.-S.; Kim, I.-S. J. Biomater. Nanobiotechnol.
2011, 2, 4.
 Guo, M.; Pitet, L. M.; Wyss, H. M.; Vos, M.; Dankers, P. Y. W.; Meijer, E. W. J. Am.
Chem. Soc. 2014, 136, 19.
 Dankers, P. Y. W.; Hermans, T. M.; Baughman, T. W.; Kamikawa, Y.; Kieltyka, R. E.;
Bastings, M. M. C.; Janssen, H. M.; Sommerdijk, N. A. J. M.; Larsen, A.; van Luyn,
M. J. A.; Bosman, A. W.; Popa, E. R.; Fytas, G.; Meijer, E. W. Adv. Mater. 2012, 24,
 Bastings, M. M. C.; Koudstaal, S.; Kieltyka, R. E.; Nakano, Y.; Pape, A. C. H.; Feyen,
D. A. M.; van Slochteren, F. J.; Doevendans, P. A.; Sluijter, J. P. G.; Meijer, E. W.;
Chamuleau, S. A. J.; Dankers, P. Y. W. Adv. Healthc. Mater. 2014, 3, 1.
 Kieltyka, R. E.; Pape, A. C. H.; Albertazzi, L.; Nakano, Y.; Bastings, M. M. C.; Voets,
I. K.; Dankers, P. Y. W.; Meijer, E. W. J. Am. Chem. Soc. 2013, 135, 30.
 Pape, A. C. H.; Bastings, M. M. C.; Kieltyka, R. E.; Wyss, H. M.; Voets, I. K.; Meijer,
E. W.; Dankers, P. Y. W. Int. J. Mol. Sci. 2014, 15, 1.
- 17 -
 Zeugolis, D. I.; Khew, S. T.; Yew, E. S. Y.; Ekaputra, A. K.; Tong, Y. W.; Yung, L. Y.
L.; Hutmacher, D. W.; Sheppard, C.; Raghunath, M. Biomaterials 2008, 29, 15.
 Huang, Z. M.; Zhang, Y. Z.; Ramakrishna, S.; Lim, C. T. Polymer 2004, 45, 15.
 Zhang, S.; Huang, Y.; Yang, X.; Mei, F.; Ma, Q.; Chen, G.; Ryu, S.; Deng, X. J.
Biomed. Mater. Res. A 2009, 90.
 Aper, S. J. A.; Van Spreeuwel, A. C. C.; Van Turnhout, M. C.; Van Der Linden, A. J.;
Pieters, P. A.; Van Der Zon, N. L. L.; De La Rambelje, S. L.; Bouten, C. V. C.; Merkx,
M. PLoS One 2014, 9, 12.
 Ryan, M. J.; Johnson, G.; Kirk, J.; Fuerstenberg, S. M.; Zager, R. A.; Torok-Storb, B.
Kidney Int. 1994, 45, 1.
 Smits, A. M.; van Vliet, P.; Metz, C. H.; Korfage, T.; Sluijter, J. P. G.; Doevendans, P.
A.; Goumans, M.-J. Nat. Protoc. 2009, 4, 2.
 Ghalbzouri, A. E.; Lamme, E.; Ponec, M. Cell Tissue Res 2002, 310.
 Browning, M. B.; Cereceres, S. N.; Luong, P. T.; Cosgriff-Hernandez, E. M. J. Biomed.
Mater. Res. - Part A 2014, 102, 4244.
 Vatankhah, E.; Semnani, D.; Prabhakaran, M. P.; Tadayon, M.; Razavi, S.;
Ramakrishna, S. Acta Biomater. 2014, 10, 2.
 Ghasemi-Mobarakeh, L.; Prabhakaran, M. P.; Morshed, M.; Nasr-Esfahani, M.-H.;
Ramakrishna, S. Biomaterials 2008, 29, 34.
 Lee, J.; Tae, G.; Kim, Y. H.; Park, I. S.; Kim, S. H.; Kim, S. H. Biomaterials 2008, 29,
 Meng, Z. X.; Wang, Y. S.; Ma, C.; Zheng, W.; Li, L.; Zheng, Y. F. Mater. Sci. Eng. C
2010, 30, 8.
 Hajiali, H.; Shahgasempour; Naimi-Jamal, M. R.; Peirovi. Int. J. Nanomedicine 2011,
 Dankers, P. Y. W.; Boomker, J. M.; Huizinga-van der Vlag, A.; Wisse, E.; Appel, W.
- 18 -
P. J.; Smedts, F. M. M.; Harmsen, M. C.; Bosman, A. W.; Meijer, W.; van Luyn, M. J.
A. Biomaterials 2011, 32, 3.
 Mollet, B. B.; Comellas-Aragonès, M.; Spiering, a. J. H.; Söntjens, S. H. M.; Meijer,
E. W.; Dankers, P. Y. W. J. Mater. Chem. B 2014, 2, 17.
 Muylaert, D. E. P.; van Almen, G. C.; Talacua, H.; Fledderus, J. O.; Kluin, J.;
Hendrikse, S. I. S.; van Dongen, J. L. J.; Sijbesma, E.; Bosman, A. W.; Mes, T.;
Thakkar, S. H.; Smits, A. I. P. M.; Bouten, C. V. C.; Dankers, P. Y. W.; Verhaar, M. C.
Biomaterials 2016, 76.
- 19 -
Figure 1: Formation of electrospun CE-UPy-PEG scaffolds in aqueous environments. (A) Chemical structure of CE-UPy-PEG and the effect of water on the nanometer-scale polymer structure, scale bars represent approximately 15 nm. (B) Photographs of a stand-alone electrospun mesh and phase contrast micrographs of a thin layer of electrospun microfibers on a glass substrate as-spun (state I) dry material, (state II) as a hydrogel after addition of cell culture media containing phenol red and (state III) dehydrated gel. Scale bars of the photographs and for the micrographs are 5 mm and 50 μm, respectively. (C) Scanning electron micrographs show the microfibrous morphology of electrospun CE-UPy-PEG meshes as-spun (state I) dry material from a solution in HFIP and (state III) after hydration and subsequent drying. Scale bars of the upper micrographs and the lower micrographs are 100 μm and 5 μm, respectively.
Figure 2: Electrospun CE-UPy-PEG with gelatin and mechanical testing of electrospun hydrogel meshes. (A) Scanning electron micrographs of dry electrospun meshes of CE-UPy-PEG with 0, 20, and 30 wt% gelatin. The scale bars indicate 50 µm. (B) Uniaxial stress-strain graphs showing one stretch-relax cycle of electrospun hydrogel meshes of CE-UPy-PEG with 0, 20 and 30 wt% gelatin in wet-state.
Table 1: Elastic moduli of electrospun CE-UPy-PEG hydrogel meshes, with and without gelatin.
Number of samples
Average fiber diameter
Average thickness a
Average E modulus b
[MPa] 100/0 N=3 0.68 ± 0.23 459 ± 36 0.64 ± 0.19 80/20 N=3 0.63 ± 0.36 374 ± 51 0.60 ± 0.15 70/30 N=2 0.65 ± 0.39 519 ± 141 0.61 ± 0.06
a Thickness of hydrated samples. b Elastic moduli were determined as the slope of the linear range of stress-strain curves. Figure 3: HK-2 adhesion and monolayer formation on electrospun hybrid meshes. (A) Fluorescence micrographs show the location of fluorescently stained gelatin in hydrated electrospun meshes of CE-UPy-PEG with 10, 20 and 30 wt% gelatin. Scale bars indicate 50 μm. (B) Fluorescence micrographs show intracellular actin of HK-2 cells 3 days after seeding on electrospun meshes of CE-UPy-PEG with 10, 20 and 30 wt% gelatin. Scale bars indicate 100 μm. (C) Immunofluorescence micrographs show cell-cell interactions with ZO-1 of HK-2 cells 3 days after seeding on electrospun meshes of CE-UPy-PEG with 10, 20 and 30 wt% gelatin. Scale bars indicate 50 μm.
Figure 4: Electrospun CE-UPy-PEG meshes and ECM production of CMPC inside electrospun hybrid meshes. (A) Scanning electron micrographs of an electrospun scaffold prepared from a concentrated solution (10 wt/v%) of CE-UPy-PEG with 20 wt% gelatin. (B) Immunofluorescence confocal micrographs show ECM production of CMPC after 1 day in the electrospun meshes. Collagen I, collagen IV and collagen III are represented in red, integrin-β1 and fibronectin are represented in green and CMPC nuclei are represented in blue.
- 20 -
TOC Mechanically robust electrospun hydrogel scaffolds crosslinked via supramolecular interactions
Elastic, bioactive supramolecular crosslinked hydrogel scaffolds are formed via electrospinning of ureido-pyrimidinone modified PEG in combination with the natural polymer gelatin. The microfibrous structure can be tuned to the application, varying from small to larger fiber diameters. Importantly, this ease of tunability resulted in microfibrous scaffolds that either support renal monolayer formation or provide a niche for cardiac progenitor cells.